#------------------------------------------------------------------------------
#$Date: 2020-11-22 01:25:53 +0200 (Sun, 22 Nov 2020) $
#$Revision: 259217 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/00/37/4003711.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4003711
loop_
_publ_author_name
'Zuluaga, Andrés Reyes'
'Brock, Aidan J.'
'Pfrunder, Michael C.'
'Phonsri, Wasinee'
'Murray, Keith S.'
'Harding, Phimphaka'
'Micallef, Aaron S.'
'Mullen, Kathleen M.'
'Clegg, Jack K.'
'Harding, David J.'
'McMurtrie, John C.'
_publ_section_title
;
 Three-Way Switchable Single-Crystal-to-Single-Crystal Solvatomorphic Spin
 Crossover in a Molecular Cocrystal
;
_journal_name_full               'Chemistry of Materials'
_journal_paper_doi               10.1021/acs.chemmater.0c03396
_journal_year                    2020
_chemical_formula_moiety         'C34 H26 Fe N4 O4, C N S, C2 H3 N'
_chemical_formula_sum            'C37 H29 Fe N6 O4 S'
_chemical_formula_weight         709.57
_chemical_name_systematic
'bis(4-methoxy-2-(((quinolin-8-yl)imino)methyl)phenolato)-iron(iii) thiocyanate acetonitrile solvate'
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_atom_sites_solution_hydrogens   geom
_audit_creation_date             2020-07-22
_audit_creation_method
;
Olex2 1.3
(compiled 2020.06.28 svn.raecde09e for OlexSys, GUI svn.r6132)
;
_cell_angle_alpha                61.702(4)
_cell_angle_beta                 83.854(3)
_cell_angle_gamma                70.058(4)
_cell_formula_units_Z            2
_cell_length_a                   12.3404(5)
_cell_length_b                   12.3475(5)
_cell_length_c                   12.5777(5)
_cell_measurement_reflns_used    13219
_cell_measurement_temperature    200.01(10)
_cell_measurement_theta_max      33.3180
_cell_measurement_theta_min      2.2840
_cell_volume                     1582.83(13)
_computing_cell_refinement       'CrysAlisPro 1.171.40.63a (Rigaku OD, 2019)'
_computing_data_collection       'CrysAlisPro 1.171.40.63a (Rigaku OD, 2019)'
_computing_data_reduction        'CrysAlisPro 1.171.40.63a (Rigaku OD, 2019)'
_computing_molecular_graphics    'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_diffrn_ambient_temperature      200.15
_diffrn_detector_area_resol_mean 5.8140
_diffrn_detector_type            'Pilatus 300K'
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_details
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  tₑₓₚ   ω     θ     κ     φ   Frames
--------------------------------------------------------------------------
  1  ω    -41.00  25.00   0.50    3.50    --   12.29 -57.00  30.00  132
  2  ω     -2.00  34.00   0.50    3.50    --   12.29 -99.00  30.00   72
  3  ω     -2.00  45.00   0.50    3.50    --   12.29 -99.00  90.00   94
  4  ω     -2.00  49.00   0.50    3.50    --   12.29 -99.00 150.00  102
  5  ω    -56.00  41.00   0.50    3.50    --   12.29 -80.00 -82.00  194
  6  ω      0.00  26.00   0.50    3.50    --   12.29 -19.00 -90.00   52
  7  ω    -15.00  15.00   0.50    3.50    --  -11.00 -80.00 -82.00   60
  8  ω     -2.00  50.00   0.50    3.50    --   12.29 -99.00 -90.00  104
  9  ω     -8.00  87.00   0.50    3.50    --   12.29  19.00-120.00  190
 10  ω     38.00  63.00   0.50    3.50    --  -11.00  57.00-180.00   50
 11  ω    -11.00  14.00   0.50    3.50    --  -11.00  57.00-180.00   50
 12  ω    -56.00 -31.00   0.50    3.50    --   12.29 -19.00 -90.00   50
 13  ω    -55.00 -25.00   0.50    3.50    --  -11.00 -80.00 -82.00   60
 14  ω     11.00  60.00   0.50    3.50    --   12.29  57.00  60.00   98
 15  ω    -16.00  41.00   0.50    3.50    --   12.29  80.00  40.00  114
 16  ω     -6.00  59.00   0.50    3.50    --   12.29  77.00 150.00  130
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'XtaLAB Synergy, Dualflex, Pilatus 300K'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0986
_diffrn_reflns_av_unetI/netI     0.0720
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            39425
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         28.282
_diffrn_reflns_theta_min         2.173
_exptl_absorpt_coefficient_mu    0.596
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.69769
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.40.63a (Rigaku Oxford Diffraction, 2019)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            'dark brown'
_exptl_crystal_colour_modifier   dark
_exptl_crystal_colour_primary    brown
_exptl_crystal_density_diffrn    1.489
_exptl_crystal_description       needle
_exptl_crystal_F_000             734
_exptl_crystal_preparation       'Combined equal ratios of starting materials'
_exptl_crystal_recrystallization_method 'Slow evaporation of the solvent'
_exptl_crystal_size_max          2
_exptl_crystal_size_mid          1
_exptl_crystal_size_min          1
_refine_diff_density_max         0.518
_refine_diff_density_min         -0.605
_refine_diff_density_rms         0.074
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.064
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     455
_refine_ls_number_reflns         7856
_refine_ls_number_restraints     26
_refine_ls_restrained_S_all      1.065
_refine_ls_R_factor_all          0.0693
_refine_ls_R_factor_gt           0.0503
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0480P)²+0.6070P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1206
_refine_ls_wR_factor_ref         0.1313
_reflns_Friedel_coverage         0.000
_reflns_number_gt                6032
_reflns_number_total             7856
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            cm0c03396_si_004.cif
_cod_data_source_block           sjcm19ar22_02_200_00
_cod_database_code               4003711
_shelx_shelxl_version_number     2018/3
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_max   0.587
_shelx_estimated_absorpt_t_min   0.382
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups
 At 1.5 times of:
  All C(H,H,H) groups
2. Restrained distances
 N7-C1A
 1.14 with sigma of 0.02
 C1A-N7
 1.137 with sigma of 0.01
 C1A-C1B
 1.456 with sigma of 0.01
 C1B-N7
 2.593 with sigma of 0.02
 N7-C1B
 2.59 with sigma of 0.04
3. Uiso/Uaniso restraints and constraints
N7 \\sim C1A \\sim C1B: within 2A with sigma of 0.04 and sigma for terminal
atoms of 0.08 within 2A
Uanis(N6) = Uanis(N7)
Uanis(C37) = Uanis(C1B)
Uanis(C36) = Uanis(C1A)
4. Rigid body (RIGU) restrains
 N7, C1A, C1B
 with sigma for 1-2 distances of 0.004 and sigma for 1-3 distances of 0.004
5. Others
 Fixed Sof: N6(0.8) C36(0.8) C37(0.8) H37A(0.8) H37B(0.8) H37C(0.8) N7(0.2)
 C1A(0.2) C1B(0.2) H1BA(0.2) H1BB(0.2) H1BC(0.2)
6.a Aromatic/amide H refined with riding coordinates:
 C25(H25), C23(H23), C6(H6), C8(H8), C2(H2), C3(H3), C20(H20), C10(H10),
 C33(H33), C19(H19), C12(H12), C27(H27), C16(H16), C11(H11), C29(H29), C28(H28),
  C15(H15), C32(H32), C14(H14), C31(H31)
6.b Idealised Me refined as rotating group:
 C22(H22A,H22B,H22C), C5(H5A,H5B,H5C), C37(H37A,H37B,H37C), C1B(H1BA,H1BB,H1BC)
;
_olex2_exptl_crystal_mounting_method 'Paratone oil'
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Fe1 Fe 0.62846(3) 0.72533(3) 0.45542(3) 0.02006(10) Uani 1 1 d . . . . .
S1 S 0.92071(8) 0.81946(11) -0.32364(9) 0.0609(3) Uani 1 1 d . . . . .
O1 O 0.55957(14) 0.64936(15) 0.60034(15) 0.0248(3) Uani 1 1 d . . . . .
O3 O 0.48791(13) 0.84803(15) 0.37175(15) 0.0243(3) Uani 1 1 d . . . . .
O4 O 0.16045(15) 0.80884(17) 0.13726(16) 0.0322(4) Uani 1 1 d . . . . .
O2 O 0.43620(16) 0.79075(18) 0.96373(16) 0.0349(4) Uani 1 1 d . . . . .
N2 N 0.70947(15) 0.80311(18) 0.30871(17) 0.0213(4) Uani 1 1 d . . . . .
N3 N 0.61935(16) 0.59139(18) 0.42054(17) 0.0212(4) Uani 1 1 d . . . . .
N4 N 0.77898(16) 0.59377(18) 0.53746(17) 0.0223(4) Uani 1 1 d . . . . .
N1 N 0.64943(16) 0.85633(18) 0.48747(17) 0.0217(4) Uani 1 1 d . . . . .
C17 C 0.74349(19) 0.9001(2) 0.3042(2) 0.0229(4) Uani 1 1 d . . . . .
C34 C 0.80147(19) 0.4810(2) 0.5291(2) 0.0232(4) Uani 1 1 d . . . . .
C9 C 0.71363(19) 0.9306(2) 0.4011(2) 0.0238(5) Uani 1 1 d . . . . .
C18 C 0.41435(19) 0.8299(2) 0.3176(2) 0.0222(4) Uani 1 1 d . . . . .
C21 C 0.2478(2) 0.8077(2) 0.1976(2) 0.0255(5) Uani 1 1 d . . . . .
C25 C 0.53152(19) 0.6002(2) 0.3644(2) 0.0226(4) Uani 1 1 d . . . . .
H25 H 0.534391 0.525755 0.357768 0.027 Uiso 1 1 calc R U . . .
C24 C 0.43158(19) 0.7129(2) 0.3121(2) 0.0229(4) Uani 1 1 d . . . . .
C26 C 0.71729(19) 0.4770(2) 0.4644(2) 0.0236(5) Uani 1 1 d . . . . .
C23 C 0.34683(19) 0.7046(2) 0.2504(2) 0.0243(5) Uani 1 1 d . . . . .
H23 H 0.359282 0.626581 0.245893 0.029 Uiso 1 1 calc R U . . .
C13 C 0.8069(2) 0.9645(2) 0.2093(2) 0.0269(5) Uani 1 1 d . . . . .
C6 C 0.5215(2) 0.8358(2) 0.7695(2) 0.0259(5) Uani 1 1 d . . . . .
H6 H 0.536469 0.908505 0.764547 0.031 Uiso 1 1 calc R U . . .
C8 C 0.6109(2) 0.8771(2) 0.5789(2) 0.0241(5) Uani 1 1 d . . . . .
H8 H 0.621863 0.948106 0.582029 0.029 Uiso 1 1 calc R U . . .
C4 C 0.4698(2) 0.7660(2) 0.8675(2) 0.0268(5) Uani 1 1 d . . . . .
C7 C 0.55324(19) 0.8013(2) 0.6748(2) 0.0226(4) Uani 1 1 d . . . . .
C2 C 0.4776(2) 0.6229(2) 0.7841(2) 0.0284(5) Uani 1 1 d . . . . .
H2 H 0.462010 0.549636 0.791173 0.034 Uiso 1 1 calc R U . . .
C3 C 0.4469(2) 0.6595(2) 0.8735(2) 0.0303(5) Uani 1 1 d . . . . .
H3 H 0.409458 0.611937 0.940655 0.036 Uiso 1 1 calc R U . . .
C1 C 0.53188(19) 0.6918(2) 0.6820(2) 0.0220(4) Uani 1 1 d . . . . .
C20 C 0.2290(2) 0.9226(2) 0.2046(2) 0.0283(5) Uani 1 1 d . . . . .
H20 H 0.159458 0.993644 0.169260 0.034 Uiso 1 1 calc R U . . .
C10 C 0.7491(2) 1.0240(2) 0.4031(2) 0.0304(5) Uani 1 1 d . . . . .
H10 H 0.730375 1.045192 0.467661 0.036 Uiso 1 1 calc R U . . .
C30 C 0.9034(2) 0.3733(2) 0.5837(2) 0.0274(5) Uani 1 1 d . . . . .
C33 C 0.8546(2) 0.6011(2) 0.5990(2) 0.0284(5) Uani 1 1 d . . . . .
H33 H 0.839204 0.679201 0.604285 0.034 Uiso 1 1 calc R U . . .
C19 C 0.3107(2) 0.9334(2) 0.2623(2) 0.0262(5) Uani 1 1 d . . . . .
H19 H 0.296798 1.012705 0.264854 0.031 Uiso 1 1 calc R U . . .
C12 C 0.8421(2) 1.0597(3) 0.2149(2) 0.0332(6) Uani 1 1 d . . . . .
H12 H 0.885793 1.104057 0.153079 0.040 Uiso 1 1 calc R U . . .
C27 C 0.7377(2) 0.3670(2) 0.4516(2) 0.0294(5) Uani 1 1 d . . . . .
H27 H 0.682965 0.363175 0.406931 0.035 Uiso 1 1 calc R U . . .
C16 C 0.7332(2) 0.7728(2) 0.2185(2) 0.0261(5) Uani 1 1 d . . . . .
H16 H 0.707922 0.707327 0.220482 0.031 Uiso 1 1 calc R U . . .
C11 C 0.8132(2) 1.0880(3) 0.3094(2) 0.0339(6) Uani 1 1 d . . . . .
H11 H 0.837031 1.152345 0.311805 0.041 Uiso 1 1 calc R U . . .
C29 C 0.9205(2) 0.2622(2) 0.5693(2) 0.0323(5) Uani 1 1 d . . . . .
H29 H 0.988376 0.188501 0.604620 0.039 Uiso 1 1 calc R U . . .
C28 C 0.8396(2) 0.2605(2) 0.5046(2) 0.0328(5) Uani 1 1 d . . . . .
H28 H 0.852486 0.185301 0.495125 0.039 Uiso 1 1 calc R U . . .
C15 C 0.7944(2) 0.8342(3) 0.1204(2) 0.0313(5) Uani 1 1 d . . . . .
H15 H 0.809500 0.810644 0.057107 0.038 Uiso 1 1 calc R U . . .
C32 C 0.9567(2) 0.4972(3) 0.6566(2) 0.0332(6) Uani 1 1 d . . . . .
H32 H 1.008776 0.505036 0.700918 0.040 Uiso 1 1 calc R U . . .
C14 C 0.8321(2) 0.9277(2) 0.1164(2) 0.0314(5) Uani 1 1 d . . . . .
H14 H 0.875249 0.968064 0.051282 0.038 Uiso 1 1 calc R U . . .
C22 C 0.1860(2) 0.7039(3) 0.1096(2) 0.0338(6) Uani 1 1 d . . . . .
H22A H 0.119422 0.715765 0.064334 0.051 Uiso 1 1 calc R U . . .
H22B H 0.203045 0.621413 0.184875 0.051 Uiso 1 1 calc R U . . .
H22C H 0.253268 0.702266 0.060527 0.051 Uiso 1 1 calc R U . . .
N5 N 0.9678(2) 0.7500(3) -0.0837(3) 0.0547(7) Uani 1 1 d . . . . .
C31 C 0.9809(2) 0.3854(3) 0.6487(2) 0.0327(5) Uani 1 1 d . . . . .
H31 H 1.050239 0.315240 0.687107 0.039 Uiso 1 1 calc R U . . .
C5 C 0.4772(2) 0.8820(3) 0.9717(2) 0.0355(6) Uani 1 1 d . . . . .
H5A H 0.445684 0.967761 0.901296 0.053 Uiso 1 1 calc R U . . .
H5B H 0.561786 0.852649 0.973260 0.053 Uiso 1 1 calc R U . . .
H5C H 0.452324 0.888086 1.045844 0.053 Uiso 1 1 calc R U . . .
N6 N 0.6977(3) 0.5689(4) 0.1389(3) 0.0549(9) Uani 0.8 1 d . . P A 1
C35 C 0.9485(2) 0.7779(3) -0.1815(3) 0.0467(8) Uani 1 1 d . . . . .
C36 C 0.7380(9) 0.5634(12) 0.0571(6) 0.0536(16) Uani 0.8 1 d . . P A 1
C37 C 0.7981(5) 0.5508(8) -0.0499(6) 0.0701(18) Uani 0.8 1 d . . P A 1
H37A H 0.742420 0.555597 -0.103301 0.105 Uiso 0.8 1 calc R U P A 1
H37B H 0.860747 0.466900 -0.021002 0.105 Uiso 0.8 1 calc R U P A 1
H37C H 0.829982 0.621818 -0.094596 0.105 Uiso 0.8 1 calc R U P A 1
N7 N 0.7918(13) 0.4886(15) 0.1699(13) 0.0549(9) Uani 0.2 1 d D U P B 2
C1A C 0.761(5) 0.545(5) 0.0687(19) 0.0536(16) Uani 0.2 1 d D U P B 2
C1B C 0.757(3) 0.577(4) -0.0598(19) 0.0701(18) Uani 0.2 1 d D U P B 2
H1BA H 0.737234 0.671803 -0.110231 0.105 Uiso 0.2 1 calc R U P B 2
H1BB H 0.698737 0.548251 -0.075398 0.105 Uiso 0.2 1 calc R U P B 2
H1BC H 0.832920 0.533315 -0.079445 0.105 Uiso 0.2 1 calc R U P B 2
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
S S 0.1246 0.1234 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 Fe1 N2 176.45(7) . . ?
O1 Fe1 N3 87.69(7) . . ?
O1 Fe1 N4 88.33(7) . . ?
O1 Fe1 N1 95.08(7) . . ?
O3 Fe1 O1 93.51(7) . . ?
O3 Fe1 N2 89.43(7) . . ?
O3 Fe1 N3 95.13(7) . . ?
O3 Fe1 N4 177.32(7) . . ?
O3 Fe1 N1 87.91(7) . . ?
N2 Fe1 N4 88.80(8) . . ?
N3 Fe1 N2 94.03(7) . . ?
N3 Fe1 N4 82.99(8) . . ?
N3 Fe1 N1 175.77(8) . . ?
N1 Fe1 N2 83.04(7) . . ?
N1 Fe1 N4 93.88(8) . . ?
C1 O1 Fe1 126.06(13) . . ?
C18 O3 Fe1 126.31(14) . . ?
C21 O4 C22 116.13(19) . . ?
C4 O2 C5 116.35(18) . . ?
C17 N2 Fe1 112.91(14) . . ?
C16 N2 Fe1 128.23(15) . . ?
C16 N2 C17 118.86(19) . . ?
C25 N3 Fe1 125.00(15) . . ?
C25 N3 C26 120.69(18) . . ?
C26 N3 Fe1 114.29(14) . . ?
C34 N4 Fe1 112.49(14) . . ?
C33 N4 Fe1 128.42(16) . . ?
C33 N4 C34 119.1(2) . . ?
C9 N1 Fe1 113.84(14) . . ?
C8 N1 Fe1 125.23(15) . . ?
C8 N1 C9 120.93(18) . . ?
N2 C17 C9 116.54(19) . . ?
N2 C17 C13 121.8(2) . . ?
C13 C17 C9 121.6(2) . . ?
N4 C34 C26 117.0(2) . . ?
N4 C34 C30 121.8(2) . . ?
C26 C34 C30 121.3(2) . . ?
C17 C9 N1 113.52(18) . . ?
C10 C9 N1 127.6(2) . . ?
C10 C9 C17 118.8(2) . . ?
O3 C18 C24 124.8(2) . . ?
O3 C18 C19 117.86(19) . . ?
C19 C18 C24 117.34(19) . . ?
O4 C21 C20 115.2(2) . . ?
C23 C21 O4 125.0(2) . . ?
C23 C21 C20 119.8(2) . . ?
N3 C25 H25 117.5 . . ?
N3 C25 C24 124.95(19) . . ?
C24 C25 H25 117.5 . . ?
C18 C24 C25 123.62(19) . . ?
C18 C24 C23 120.0(2) . . ?
C25 C24 C23 116.33(19) . . ?
C34 C26 N3 113.24(18) . . ?
C27 C26 N3 128.0(2) . . ?
C27 C26 C34 118.8(2) . . ?
C21 C23 C24 120.6(2) . . ?
C21 C23 H23 119.7 . . ?
C24 C23 H23 119.7 . . ?
C17 C13 C12 117.8(2) . . ?
C17 C13 C14 117.4(2) . . ?
C14 C13 C12 124.8(2) . . ?
C4 C6 H6 119.5 . . ?
C4 C6 C7 121.1(2) . . ?
C7 C6 H6 119.5 . . ?
N1 C8 H8 117.6 . . ?
N1 C8 C7 124.85(19) . . ?
C7 C8 H8 117.6 . . ?
O2 C4 C3 115.2(2) . . ?
C6 C4 O2 125.7(2) . . ?
C6 C4 C3 119.2(2) . . ?
C6 C7 C8 116.69(19) . . ?
C6 C7 C1 119.8(2) . . ?
C1 C7 C8 123.46(19) . . ?
C3 C2 H2 119.3 . . ?
C3 C2 C1 121.4(2) . . ?
C1 C2 H2 119.3 . . ?
C4 C3 H3 119.4 . . ?
C2 C3 C4 121.2(2) . . ?
C2 C3 H3 119.4 . . ?
O1 C1 C7 125.0(2) . . ?
O1 C1 C2 117.54(18) . . ?
C2 C1 C7 117.45(19) . . ?
C21 C20 H20 119.7 . . ?
C19 C20 C21 120.5(2) . . ?
C19 C20 H20 119.7 . . ?
C9 C10 H10 120.0 . . ?
C9 C10 C11 120.0(2) . . ?
C11 C10 H10 120.0 . . ?
C29 C30 C34 118.2(2) . . ?
C31 C30 C34 117.1(2) . . ?
C31 C30 C29 124.7(2) . . ?
N4 C33 H33 119.0 . . ?
N4 C33 C32 122.1(2) . . ?
C32 C33 H33 119.0 . . ?
C18 C19 H19 119.2 . . ?
C20 C19 C18 121.7(2) . . ?
C20 C19 H19 119.2 . . ?
C13 C12 H12 119.9 . . ?
C11 C12 C13 120.1(2) . . ?
C11 C12 H12 119.9 . . ?
C26 C27 H27 120.0 . . ?
C26 C27 C28 120.0(2) . . ?
C28 C27 H27 120.0 . . ?
N2 C16 H16 118.9 . . ?
N2 C16 C15 122.3(2) . . ?
C15 C16 H16 118.9 . . ?
C10 C11 H11 119.2 . . ?
C12 C11 C10 121.6(2) . . ?
C12 C11 H11 119.2 . . ?
C30 C29 H29 120.0 . . ?
C28 C29 C30 119.9(2) . . ?
C28 C29 H29 120.0 . . ?
C27 C28 H28 119.1 . . ?
C29 C28 C27 121.9(2) . . ?
C29 C28 H28 119.1 . . ?
C16 C15 H15 120.2 . . ?
C14 C15 C16 119.7(2) . . ?
C14 C15 H15 120.2 . . ?
C33 C32 H32 120.1 . . ?
C31 C32 C33 119.8(2) . . ?
C31 C32 H32 120.1 . . ?
C13 C14 H14 120.1 . . ?
C15 C14 C13 119.9(2) . . ?
C15 C14 H14 120.1 . . ?
O4 C22 H22A 109.5 . . ?
O4 C22 H22B 109.5 . . ?
O4 C22 H22C 109.5 . . ?
H22A C22 H22B 109.5 . . ?
H22A C22 H22C 109.5 . . ?
H22B C22 H22C 109.5 . . ?
C30 C31 H31 119.9 . . ?
C32 C31 C30 120.2(2) . . ?
C32 C31 H31 119.9 . . ?
O2 C5 H5A 109.5 . . ?
O2 C5 H5B 109.5 . . ?
O2 C5 H5C 109.5 . . ?
H5A C5 H5B 109.5 . . ?
H5A C5 H5C 109.5 . . ?
H5B C5 H5C 109.5 . . ?
N5 C35 S1 179.5(3) . . ?
N6 C36 C37 177.1(7) . . ?
C36 C37 H37A 109.5 . . ?
C36 C37 H37B 109.5 . . ?
C36 C37 H37C 109.5 . . ?
H37A C37 H37B 109.5 . . ?
H37A C37 H37C 109.5 . . ?
H37B C37 H37C 109.5 . . ?
N7 C1A C1B 159(4) . . ?
C1A C1B H1BA 109.5 . . ?
C1A C1B H1BB 109.5 . . ?
C1A C1B H1BC 109.5 . . ?
H1BA C1B H1BB 109.5 . . ?
H1BA C1B H1BC 109.5 . . ?
H1BB C1B H1BC 109.5 . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Fe1 O1 1.8751(16) . ?
Fe1 O3 1.8702(16) . ?
Fe1 N2 1.9765(19) . ?
Fe1 N3 1.9405(17) . ?
Fe1 N4 1.9791(19) . ?
Fe1 N1 1.9421(17) . ?
S1 C35 1.649(4) . ?
O1 C1 1.327(2) . ?
O3 C18 1.324(2) . ?
O4 C21 1.376(3) . ?
O4 C22 1.423(3) . ?
O2 C4 1.374(3) . ?
O2 C5 1.429(3) . ?
N2 C17 1.374(3) . ?
N2 C16 1.331(3) . ?
N3 C25 1.303(3) . ?
N3 C26 1.414(3) . ?
N4 C34 1.377(3) . ?
N4 C33 1.326(3) . ?
N1 C9 1.420(3) . ?
N1 C8 1.302(3) . ?
C17 C9 1.416(3) . ?
C17 C13 1.413(3) . ?
C34 C26 1.413(3) . ?
C34 C30 1.414(3) . ?
C9 C10 1.377(3) . ?
C18 C24 1.421(3) . ?
C18 C19 1.409(3) . ?
C21 C23 1.366(3) . ?
C21 C20 1.401(3) . ?
C25 H25 0.9500 . ?
C25 C24 1.423(3) . ?
C24 C23 1.425(3) . ?
C26 C27 1.378(3) . ?
C23 H23 0.9500 . ?
C13 C12 1.418(3) . ?
C13 C14 1.413(3) . ?
C6 H6 0.9500 . ?
C6 C4 1.368(3) . ?
C6 C7 1.421(3) . ?
C8 H8 0.9500 . ?
C8 C7 1.428(3) . ?
C4 C3 1.402(3) . ?
C7 C1 1.423(3) . ?
C2 H2 0.9500 . ?
C2 C3 1.374(3) . ?
C2 C1 1.411(3) . ?
C3 H3 0.9500 . ?
C20 H20 0.9500 . ?
C20 C19 1.379(3) . ?
C10 H10 0.9500 . ?
C10 C11 1.408(3) . ?
C30 C29 1.410(3) . ?
C30 C31 1.410(3) . ?
C33 H33 0.9500 . ?
C33 C32 1.404(3) . ?
C19 H19 0.9500 . ?
C12 H12 0.9500 . ?
C12 C11 1.371(4) . ?
C27 H27 0.9500 . ?
C27 C28 1.405(3) . ?
C16 H16 0.9500 . ?
C16 C15 1.404(3) . ?
C11 H11 0.9500 . ?
C29 H29 0.9500 . ?
C29 C28 1.366(4) . ?
C28 H28 0.9500 . ?
C15 H15 0.9500 . ?
C15 C14 1.364(3) . ?
C32 H32 0.9500 . ?
C32 C31 1.359(4) . ?
C14 H14 0.9500 . ?
C22 H22A 0.9800 . ?
C22 H22B 0.9800 . ?
C22 H22C 0.9800 . ?
N5 C35 1.137(4) . ?
C31 H31 0.9500 . ?
C5 H5A 0.9800 . ?
C5 H5B 0.9800 . ?
C5 H5C 0.9800 . ?
N6 C36 1.115(9) . ?
C36 C37 1.513(8) . ?
C37 H37A 0.9800 . ?
C37 H37B 0.9800 . ?
C37 H37C 0.9800 . ?
N7 C1A 1.154(9) . ?
C1A C1B 1.472(10) . ?
C1B H1BA 0.9800 . ?
C1B H1BB 0.9800 . ?
C1B H1BC 0.9800 . ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
Fe1 O1 C1 C7 -2.0(3) . . . . ?
Fe1 O1 C1 C2 178.34(16) . . . . ?
Fe1 O3 C18 C24 -1.4(3) . . . . ?
Fe1 O3 C18 C19 178.00(15) . . . . ?
Fe1 N2 C17 C9 -1.5(3) . . . . ?
Fe1 N2 C17 C13 177.36(17) . . . . ?
Fe1 N2 C16 C15 -178.35(18) . . . . ?
Fe1 N3 C25 C24 4.7(3) . . . . ?
Fe1 N3 C26 C34 2.0(2) . . . . ?
Fe1 N3 C26 C27 -178.3(2) . . . . ?
Fe1 N4 C34 C26 0.6(2) . . . . ?
Fe1 N4 C34 C30 -178.66(17) . . . . ?
Fe1 N4 C33 C32 177.55(18) . . . . ?
Fe1 N1 C9 C17 3.8(2) . . . . ?
Fe1 N1 C9 C10 -175.4(2) . . . . ?
Fe1 N1 C8 C7 4.3(3) . . . . ?
O1 Fe1 O3 C18 -84.81(18) . . . . ?
O3 Fe1 O1 C1 -83.33(18) . . . . ?
O3 C18 C24 C25 -0.3(4) . . . . ?
O3 C18 C24 C23 -179.5(2) . . . . ?
O3 C18 C19 C20 -179.6(2) . . . . ?
O4 C21 C23 C24 -179.3(2) . . . . ?
O4 C21 C20 C19 -179.7(2) . . . . ?
O2 C4 C3 C2 -179.0(2) . . . . ?
N2 Fe1 O3 C18 97.17(18) . . . . ?
N2 C17 C9 N1 -1.5(3) . . . . ?
N2 C17 C9 C10 177.8(2) . . . . ?
N2 C17 C13 C12 -177.6(2) . . . . ?
N2 C17 C13 C14 1.5(3) . . . . ?
N2 C16 C15 C14 0.4(4) . . . . ?
N3 Fe1 O1 C1 -178.33(18) . . . . ?
N3 Fe1 O3 C18 3.17(18) . . . . ?
N3 C25 C24 C18 -1.6(4) . . . . ?
N3 C25 C24 C23 177.7(2) . . . . ?
N3 C26 C27 C28 -178.3(2) . . . . ?
N4 Fe1 O1 C1 98.62(18) . . . . ?
N4 C34 C26 N3 -1.7(3) . . . . ?
N4 C34 C26 C27 178.5(2) . . . . ?
N4 C34 C30 C29 -179.1(2) . . . . ?
N4 C34 C30 C31 0.7(3) . . . . ?
N4 C33 C32 C31 0.8(4) . . . . ?
N1 Fe1 O1 C1 4.88(19) . . . . ?
N1 Fe1 O3 C18 -179.77(18) . . . . ?
N1 C9 C10 C11 179.6(2) . . . . ?
N1 C8 C7 C6 177.5(2) . . . . ?
N1 C8 C7 C1 0.5(4) . . . . ?
C17 N2 C16 C15 1.7(3) . . . . ?
C17 C9 C10 C11 0.5(4) . . . . ?
C17 C13 C12 C11 -0.8(4) . . . . ?
C17 C13 C14 C15 0.6(4) . . . . ?
C34 N4 C33 C32 -0.4(3) . . . . ?
C34 C26 C27 C28 1.4(4) . . . . ?
C34 C30 C29 C28 -0.3(4) . . . . ?
C34 C30 C31 C32 -0.3(4) . . . . ?
C9 N1 C8 C7 -175.1(2) . . . . ?
C9 C17 C13 C12 1.2(3) . . . . ?
C9 C17 C13 C14 -179.7(2) . . . . ?
C9 C10 C11 C12 -0.1(4) . . . . ?
C18 C24 C23 C21 -0.9(3) . . . . ?
C21 C20 C19 C18 -1.0(4) . . . . ?
C25 N3 C26 C34 -176.53(19) . . . . ?
C25 N3 C26 C27 3.2(4) . . . . ?
C25 C24 C23 C21 179.8(2) . . . . ?
C24 C18 C19 C20 -0.2(3) . . . . ?
C26 N3 C25 C24 -176.9(2) . . . . ?
C26 C34 C30 C29 1.6(3) . . . . ?
C26 C34 C30 C31 -178.5(2) . . . . ?
C26 C27 C28 C29 -0.1(4) . . . . ?
C23 C21 C20 C19 1.3(4) . . . . ?
C13 C17 C9 N1 179.7(2) . . . . ?
C13 C17 C9 C10 -1.0(3) . . . . ?
C13 C12 C11 C10 0.3(4) . . . . ?
C6 C4 C3 C2 1.3(4) . . . . ?
C6 C7 C1 O1 -178.8(2) . . . . ?
C6 C7 C1 C2 0.9(3) . . . . ?
C8 N1 C9 C17 -176.8(2) . . . . ?
C8 N1 C9 C10 4.0(4) . . . . ?
C8 C7 C1 O1 -1.9(4) . . . . ?
C8 C7 C1 C2 177.8(2) . . . . ?
C4 C6 C7 C8 -177.6(2) . . . . ?
C4 C6 C7 C1 -0.5(4) . . . . ?
C7 C6 C4 O2 179.7(2) . . . . ?
C7 C6 C4 C3 -0.7(4) . . . . ?
C3 C2 C1 O1 179.5(2) . . . . ?
C3 C2 C1 C7 -0.2(4) . . . . ?
C1 C2 C3 C4 -0.9(4) . . . . ?
C20 C21 C23 C24 -0.3(4) . . . . ?
C30 C34 C26 N3 177.6(2) . . . . ?
C30 C34 C26 C27 -2.2(3) . . . . ?
C30 C29 C28 C27 -0.4(4) . . . . ?
C33 N4 C34 C26 178.9(2) . . . . ?
C33 N4 C34 C30 -0.4(3) . . . . ?
C33 C32 C31 C30 -0.5(4) . . . . ?
C19 C18 C24 C25 -179.6(2) . . . . ?
C19 C18 C24 C23 1.2(3) . . . . ?
C12 C13 C14 C15 179.6(2) . . . . ?
C16 N2 C17 C9 178.5(2) . . . . ?
C16 N2 C17 C13 -2.6(3) . . . . ?
C16 C15 C14 C13 -1.6(4) . . . . ?
C29 C30 C31 C32 179.6(2) . . . . ?
C14 C13 C12 C11 -179.8(2) . . . . ?
C22 O4 C21 C23 -12.1(3) . . . . ?
C22 O4 C21 C20 168.9(2) . . . . ?
C31 C30 C29 C28 179.8(2) . . . . ?
C5 O2 C4 C6 -11.7(4) . . . . ?
C5 O2 C4 C3 168.7(2) . . . . ?
